INTERNATIONAL WELDING SPECIALIST (IWS) INCORPORATING WTIA WELDING SUPERVISOR AS 1796 CERTIFICATE 10 AND AS 2214 WELDING SUPERVISORAND INTERNATIONAL WELDING INSPECTION PERSONNEL STANDARD (IWI S) INCORPORATING WTIA WELDING INSPECTOR SAMPLE QUESTIONS AND ANSWERS BANK Page 1 of 23 Rev 1 QUESTION 1 1.1 State five functions of the flux in the flux cored arc welding process. • • • • • Stabilise the arc Shield molten metal from atmosphere Scavenge impurities Controls shape and appearance of weld Adjusts chemical composition of weld 5 marks (Ref: 1.8) 1.2 With the aid of diagrams, briefly explain the difference between Constant Current and Constant Voltage welding power sources. 10 marks (Ref: 1.5, 1.8, 1.9) Voltage Voltage Current CONSTANT CURRENT Current CONSTANT VOLTAGE Welding machines are usually classified as constant current (CC) or constant voltage (CV). A constant current machine will vary its output voltage to maintain a steady current while a constant voltage machine will fluctuate its output current to maintain a set voltage. Shielded metal arc welding use a constant current source and gas metal arc welding and flux-cored arc welding typically use constant voltage sources 1.3 List the four main modes of metal transfer in Gas Metal Arc Welding (GMAW) process. 5 marks (Ref: 1.8) • • • • Short circuiting transfer Globular transfer Spray Transfer Pulsed spray transfer Page 2 of 23 Rev 1 10) It improves the current pickup between contact tip and the electrode.2 5 marks (Ref: 1. the information conveyed through it.3 Given the welding symbol as shown below. 7 marks (Ref: 1. alternatively 2. What is “twin wire” (tandem wire) GMAW? What are the two variations in the welding process? 8 marks (Ref: 1. It aids in the drawing process Helps prevent rusting of the wire when it is exposed to the atmosphere.QUESTION 2 2.1 List three reasons why SAW solid wires are copper coated.8) Automated GMAW process with two wires under one shielding gas nozzle. The lead wire generates the required penetration while the trail wire provides additional joint filling as well as an excellent weld profile. Welding current may be pulsed or non-pulsed. The tips are insulated from one another and connected to their own wire feeder and power source and regulated by electronic control system. • • • 2. Variation 1: The lead wire uses non-pulsed current. while the trailing wire uses pulsed current Variation 2: Pulsed current is applied to both wires.1) 5 50-100 • • • • • Fillet weld on one side of the joint Stitch welding Fillet leg length : 5 mm Length of fillet weld: 50 mm Pitch between welds : 100 mm Page 3 of 23 Rev 1 . explain in full with the aid of a diagram. testing requirement. c) Deposition efficiency (for continuous electrodes) 4 marks Deposition efficiency in arc welding is the ratio of the weight of the weld metal deposited to the nett weight of the filler material used.1 Define the following welding terms: Open circuit voltage of a welding power source (Ref: 1.100mm 5 mm 5050 50 mm QUESTION 3 3. The voltage is impressed upon the circuit. finish. and inspectors. Page 4 of 23 Rev 1 . however. b) Operator duty cycle 4 marks Operator duty cycle is the actual time an operator is actually welding versus time spent on related activities such as set up. No current flows in the circuit because the circuit is open. current is DC with electrode negative.1) 4 marks a) A welding machine that is turned on but not being used for welding at the moment will have a voltage applied to the cables attached to the output terminals of the welding machine. dimensions etc e) Polarity 4 marks Polarity refers to the manner in which the electrode holder and workpiece connections are connected to the electrical supply. for example. the current will flow immediately. supervisors. edge preparation. d) Welding symbol 4 marks Welding symbols are a simple way of communicating design office details to a number of different industrial shop floor personnel such as welders. clean up or some other non-welding activities. so that when the circuit is completed. Information provided by a welding symbol include weld type. In DCEN polarity. quench the flame produced by a flashback and may provide additional protection by shutting off the gas flow if certain temperatures and/or pressures are exceeded.1 What is magnetic arc blow? State three methods of reducing it.1) Soldering is a group of joining processes that produce coalescence of materials by heating them to the soldering temperature and by using a filler metal (solder) having a liquidus not exceeding 450ºC. hoses. to one side. A flashback arrestor is designed to prevent the backflow of gas. mixing of gases in torch. 1. fusion takes place with melting of both the base metal and usually a filler metal. occurs in DC arc welding when the arc does not follow the shortest path between the electrode and the workpiece and deflects forward or backward from the direction of travel or less frequently.3 What are Voltage Reducing Devices (VRDs)? List the three types of VRDs commonly used in the industry.1 Explain the difference between soldering and welding. The three types of VRDs are: Type 1: Externally fitted to secondary circuit Type 2: Internally fitted to secondary circuit Type 3: Fitted to primary circuit QUESTION 5 5.9) Magnetic arc blow. the Open Circuit Voltage is returned to a safe value until the next welding cycle. A flashback is the flame burning back into the torch. 8 marks (Ref: 1.2) Unequal gas pressure can lead to a backflow i. hoses etc that can result in a flashback. How does a flashback arrestor assist in preventing flashbacks? 7 marks (Ref: 1.QUESTION 4 4. Upon arc strike.e.8. Some of the methods to reduce it are: • • If DC is being used with MMAW process change to AC Hold as short an arc as possible to help arc force counteract arc blow Page 5 of 23 Rev 1 . 5 marks (Ref: 1. Upon completion of welding. In welding. 5 marks (Ref: 1. It is a device that reduces open-circuit voltage to a safe value until welding commences. 4. full selected current and voltage becomes available. 4.8) A device that assists in the reduction of electrical shock to personnel involved in welding activities is known as VRD. also called arc wandering.2 Explain the phenomenon of “flashback”. and below the solidus of the base metals. regulator or even the cylinders. the weld area is overheated. Abrasive jets can machine thicker materials. such as Aluminum and Copper. Abrasive jets are more environmentally friendly. No burnt fingers.3 Explain the principles of Flash Butt Welding with neat sketches. no noxious fumes and no fires. Capital equipment costs for water jet are generally much lower than that for a laser.2 Give five advantages of waterjet cutting over LASER cutting. Abrasive jets are safer. The weld is then completed by application of sufficient forging pressure and the interruption of current.12) 5. Flash butt welding is done by placing two work parts in the jaws of the flash butt machine. Abrasive jets do not heat the part. though probably just as frequent. sufficient heat is generated in the parts and it is impossible to obtain the proper upset. Maintenance on the abrasive jet nozzle is simpler than that of a laser. If it is too long. It is therefore difficult to expel the excessive molten metal and maintain an adequate forging force. This is the total time during which the flashing takes place.12) 5. Thus there is no thermal distortion or hardening of the material.• • • • Reduce the welding current Angle the electrode with the work opposite to the direction of arc blow Use a backstep welding method Wrap the work cable around the workpiece so that the current returning to the power supply passes through it in such a direction that the magnetic field set up neutralises the magnetic field causing the arc blow 5 marks (Ref: 1. The overall flashing time is important. As the parts are brought together into very light contact. (Reflective materials in particular. Modern Abrasive jets are typically much easier to operate and maintain than lasers Abrasive jets don't create "scaley" edges. a voltage is applied which produces a flashing action between work parts. which makes it easier to make a high quality weld 5 marks (Ref: 1. Flashing continues as the parts advance until the parts reach a forging temperature. If the time is too short. Page 6 of 23 Rev 1 . • • • • • • • • • • • Abrasive waterjets can machine many materials that lasers cannot. Precision abrasive jet machines can obtain about the same or higher tolerances than lasers (especially as thickness increases).) Uniformity of material is not very important to an Abrasive jet. By reducing spatter. because excessive heating tends to cause expulsion of the zinc coating under the electrodes. In general. extremely high welding current is to be avoided. it increases process efficiency and minimizes cleanup Page 7 of 23 Rev 1 . resistance welding is preferred for joining galvanised sheet products because it results in less fuming than other types of welding. The right wire size and type. the more fumes are generated. 5 marks (Ref: 1.9) For metal arc welding and other high temperature welding methods. High levels of spatter and welding fume and poor bead shape are common. precautions must be taken to avoid porosity and cracking of the weld that can be caused by penetration of zinc into the weld pool. For all galvanised products. can substantially improve gas metal arc welding (GMAW) performance on galvanized and coated steels.4 List two problems with welding coated steels and give one solution for each problem. matched with the most appropriate shielding gas.8. 1. The thicker the zinc coating. The optimum setting of the welding parameters must be determined by trial and are dependent on the specific application and sheet characteristics such as thickness or coating weight. Pulsed metal transfer GMAW can help improve galvanized steel weld quality even more.Schematic representation of flash butt welding 5. preheat = 1500 C Page 8 of 23 Rev 1 . MMAW is to be used throughout using 5 mm diameter E 4818 electrodes. calculate the arc energy Arc Voltage = 23 V.587 kJ iii) a) Using the above information and results.22% 1. 2.7.40% 0. Travel Speed = 200 mm/min 5 marks Arc Energy = (Voltage x Current) / Travel Speed = (230x23)/200 = 1.1 A steel.PAPER SA2 MATERIALS AND THEIR BEHAVIOUR DURING WELDING QUESTION 1 2. determine from the welding data sheets provided The group number of this steel 5 marks Using the graph in Fig 1 in WTIA Tech Note 1. with the chemical composition as shown below.8.614 5 marks ii) For the welding conditions given below.9) 20 All dimensions in mms C Mn Ni Cr Mo V Cu 0. 2. (Note: Use WTIA Technote 1:The Weldability of Steels for solving this problem) i) Calculate the carbon equivalent for this steel Using the IIW formula below and substituting the values: Ceq = C + Mn/6 + (Cr + Mo + V)/5 + (Ni + Cu)/15 = 0.01% 250 20 100 100 Continuous fillet welds have to be made simultaneously on a Tee Joint whose thickness is 20 mm. Amperage = 230 A.20% 0.20% 0. welding conditions and electrode size Using the graph in Fig 3 in WTIA Tech Note 1.25% 0.20% 0. Group No is 8 b) The preheat necessary for control of HAZ properties of this steel to avoid cold cracking with 5 marks the given joint configuration. and of known heat analysis.604 +0.01 = 0. (Ref: 2. is to be used in structural fabrication. Large weld beads are undesirable.2 Give four precautions that can assist in re-heat cracking being avoided in low alloy steels. such as partial penetration welds. and therefore will be more susceptible to reheat cracking. 10 marks (Ref: 2. joints likely to contain stress concentration. and in the coarse grained regions within the weld metal. usually associated with areas of stress concentration such as the weld toe. sulphur. The presence of impurities which segregate to the grain boundaries and promote temper embrittlement. Steel choice: If possible. The joint design can increase the risk of cracking. Welding procedure and technique: The welding procedure can be used to minimise the risk of reheat cracking by * Producing the maximum refinement of the coarse grain HAZ * Limiting the degree of austenite grain growth * Eliminating stress concentrations Page 9 of 23 Rev 1 . Cracking is almost exclusively found in the coarse grained regions of the heat affected zone (HAZ) beneath the weld. as they produce a coarse grained HAZ which is less likely to be refined by the subsequent pass. will increase the susceptibility to reheat cracking. vanadium and molybdenum when the welded component is being subjected to post weld heat treatment. tin and phosphorus. such as stress relief heat treatment. or cladding.1 What is re-heat cracking? Explain the reasons why re-heat cracking occurs in low alloy 10 marks (Ref: 2. are more liable to initiate cracks. or has been subjected to high temperature service (typically 350 to 550°C). For example.QUESTION 2 2. The principal cause is that when heat treating susceptible steels. arsenic. The welding procedure also has an influence. the grain interior becomes strengthened by carbide precipitation. The cracks can often be seen visually. avoid welding steels known to be susceptible to reheat cracking. 2. e.11) steels Reheat cracking may occur in low alloy steels containing alloying additions of chromium. forcing the relaxation of residual stresses by creep deformation at the grain boundaries. specifying the maximum impurity level and by adopting a more tolerant welding procedure / technique.11) The risk of reheat cracking can be reduced through the choice of steel.g. 10 marks (Ref: 2. Chemical etching: A solution of 5% sodium hydroxide can be used for batch cleaning but this should be followed by rinsing in HNO 3 and water to remove reaction products on the surface. Mechanical cleaning: Wire brushing (stainless steel bristles). solvent degreasing and chemical etch cleaning. Three cleaning techniques are suitable.QUESTION 3 3. Page 10 of 23 Rev 1 . rigorous cleaning of material surface and filler wire should be carried out. The factors that affect the final composition are: • • • The type of process being used The parameters being used by the process The nature of the base and filler materials QUESTION 4 4.4) It is a two-dimensional graph which indicates the phases present at a given temperature and composition.1 The risk of porosity during the welding of aluminium and aluminium alloys can be minimised by rigorous cleaning of material surface and filler wires used.25) Dilution of filler material by the infusion of parent metal during liquidus state in welding is a fundamental process of welding and can be defined as the reduction in alloy content of a weld deposit by virtue of melting and incorporating melted base metal of lower alloy content Dilution is commonly expressed as the percentage of base metal that has entered into the weld metal. mechanical cleaning. 8 marks (Ref: 2. scraping or filing can be used to remove surface oxide and contaminants. spraying or wiping with organic solvents can be used to remove grease. 3.1 What is a phase diagram (also called equilibrium diagram or constitution diagram)? Give two uses of the iron-carbon equilibrium diagram.23) To minimise the risk.2 How is dilution of filler material defined and expressed? What are the factors that effect the final chemical composition and mechanical/physical properties of the welded joint? 10 marks (Ref: 2. dirt and loose particles. Solvents: Dipping. Explain the three cleaning techniques that are available for achieving this. Degreasing should be carried out before mechanical cleaning. oil. the deformation may become so large that a component can no longer perform its function QUESTION 5 5. Creep does not happen upon sudden loading but the accumulation of creep strain in longer times causes failure of the material. If pitting conditions exist. the material permanently strains over a longer period of time until it finally fails. development of corrosion pits will introduce additional points of stress concentration at which cracking may develop.14) Creep is the term given to the material deformation that occurs as a result of long term exposure to levels of stress that are below the yield or ultimate strength. 12 marks (Ref: 2. 4. Page 11 of 23 Rev 1 . a liquid.1 What is the effect of corrosion on the fatigue strength of welded structures? 6 marks (Ref: 2. To find the combinations of temperature and pressure at which two states are in equilibrium. describe the phenomenon of creep.• • To get some idea of the conditions of temperature and pressure that are most likely to produce a gas. Depending on the magnitude of the applied stress and its duration. This makes creep deformation a "timedependent" deformation of the material. The rate of this damage is a function of the material properties and the exposure time. Rather than failing suddenly with a fracture. State three elements that contribute to the rate of creep damage. or a solid.2 With the aid of a diagram .15) The presence of a corrosive environment may accelerate fatigue crack propagation in structural steels. exposure temperature and the applied load (stress). Both these mechanisms are likely to reduce fatigue strength below that in an inert environment. The choice of method of applying preheat will depend on the material thickness.2 Give two reasons why preheat is used when welding a high carbon equivalent steel? List two methods of applying preheat.3 a) List two specific imperfections that can result in the welding of each of the following: Austenitic stainless steel 4 marks (Ref: 2. Si. weldment size and the heating equipment available at the time of welding. high oxygen content leads to embrittlement in the heat affected zone (HAZ) and weld metal porosity. Preheat can be applied through various means. b) Copper and copper alloys 4 marks (Ref: 2. weld metal and HAZ cracking can occur. 2. electrical strip heaters.16) Common imperfections found on welding are: Although austenitic stainless steel is readily welded. The methods can include furnace heating for small production assemblies or. Mn. It is used for the following main reasons: • To slow the cooling rate of the weld and the base material. Page 12 of 23 Rev 1 . P and Ti).5. 6 marks (Ref: 2. Weld metal solidification cracking is more likely in fully austenitic structures which are more crack sensitive than those containing a small amount of ferrite. arrays of torches. Porosity is best avoided by using appropriate filler wire containing deoxidants (Al. for large structural components.21) In fusion welding tough pitch copper. The reduction in hydrogen reduces the risk of cracking. Phosphorus deoxidised copper is more weldable but residual oxygen can result in porosity in autogenous welds especially in the presence of hydrogen. • 5.8.9) Preheating is the process applied to raise the temperature of the parent steel before welding. The slower cooling rate encourages hydrogen diffusion from the weld area by extending the time period over which it is at elevated temperature (particularly the time at temperatures above approximately 100°C) at which temperatures hydrogen diffusion rates are significantly higher than at ambient temperature. resulting in softer weld metal and heat affected zone microstructures with a greater resistance to fabrication hydrogen cracking. induction heaters or radiation heaters. 4) What is meant by “joint efficiency” Joint efficiency is the ratio between the tensile strength of the joint and the tensile strength of the parent material expressed as a percentage 1.3. 3. which is under tension.2 Define the “design throat thickness” and “load carrying area” for a fillet weld 8 marks Design throat thickness is the shortest distance from the root of the fillet weld to the line drawn between the toes of the weld.2.3 Graphically represent the actual stress distribution around the hole in the plate shown. The load carrying area is the design throat thickness multiplied by the length of the weld.PAPER SA3 CONSTRUCTION AND DESIGN QUESTION 1 1.1 5 marks ( Ref: 3. 3. 7 marks Page 13 of 23 Rev 1 .1. 3. 1. 2 single vee butt weld with convex profile double vee butt weld flushed off both sides on weld face single bevel butt weld flushed double bevel butt convex (as welded) concave fillet weld double sided convex fillet weld What is the “Poisson's ratio” and what does it indicate? 8 marks (Ref: 3.1 Find the weld throat size and the weld throat shear stress of the given fillet weld.QUESTION 2 2. it tends to get thinner in the other two directions.1 Given below are a few welding symbols. for the given information: 12 marks (Ref: 3. Poisson's ratio (ν) is a measure of this tendency.4) 12 marks a) b) c) d) e) f) 2.1) When a sample of material is stretched in one direction. It is defined as the ratio of the strain in the direction of the applied load to the strain normal to the load.4) Leg length Longitudinal shear load Weld length = 10 mm (equal legs) = 1500 N = 100 mm Page 14 of 23 Rev 1 . as shown below. QUESTION 3 3. Describe what each symbol represents (Ref: 3. 707 x 10 = 7.9) Magnitude of stress including stress concentrations caused by part geometry. This stress build up is called residual stress.1 How are residual stresses caused? 5 marks (Ref: 3.2 • State at least five factors that affect fatigue life. stresses are locked into the local weld areas.4) • • • • • • Load requirements Least amount of weld material Reduce residual internal stresses Reduce distortion Reduce cost Decrease welding time QUESTION 4 4.Throat size = Sin 450 x 10 mm = 0.07 mm Weld throat shear stress = Load/ area = 1500 /100 x 7.2 What factors (give at least five) are taken into account when selecting/designing a joint for an application 8 marks (Ref: 3. How does shot peening improve fatigue life? 10 marks (Ref: 3. 4. Because the surrounding parent metal restricts free expansion and contraction during heating and cooling cycle.12 N/mm2 3. Page 15 of 23 Rev 1 .07 = 2. the grain sizes are changed in the weld zone. Residual stress can also be caused by cold working material such as bending or rolling plates.7) Because of the high localised heat input of the welding process. the direction of the applied stress can affect fatigue life. Significantly uneven cooling. of how the designer can reduce distortion at the design stage. in the case of alloys. can significantly impact fatigue life. for most metals.3 What significant properties does “9% Ni steel” have and what applications is it used for ? 5 marks ( Ref: 3. frequency. gouges. 3. Other alloy steels are suitable for service in the lowtemperature range. It is satisfactory for service down to -195°C and is used for transport and storage of cryogenics because of its low cost and ease of fabrication. Environmental conditions and exposure time can cause erosion. and nickel steels with 3. and location of surface defects such as scratches.5% Ni to -101°C. Shot peening puts the surface in a state of compressive stress which inhibits crack formation thus improving fatigue life 4. Casting defects such as gas porosity and shrinkage voids. scratches. The steels A201 and T-1 can suffice to -45°C.6.25% Ni can suffice to -59°C. and location of internal defects. nickel steels with 2. surface roughness. copper.) strain rate also affects fatigue life in low-cycle fatigue situations.• • • • • • • Quality of the surface. titanium. shape. Surface defect geometry and location. leading to a heterogeneous distribution of material properties such as hardness and ductility and. Grain size. The size. fine-grained parts exhibit a longer fatigue life than coarsegrained parts. In metals where strain-rate sensitivity is observed (ferrous metals.1 Give five examples. or gas-phase embrittlement. Size. with sketches. etc.10) The only alloy steel recommended for cryogenic service is 9% nickel steel. which all affect fatigue life. 10 marks (Ref: 3. For non-isotropic materials. structural composition. and dents can have a significant impact on fatigue life. for example. etc.4) Avoid excessive reinforcement Reduce bevel angle and use larger root opening Page 16 of 23 Rev 1 . QUESTION 5 5. corrosion. cause stress concentrations or provide crack nucleation sites which can lower fatigue life depending on how the stress is applied. Preset parts Weld near neutral axis 1 1 2 3 Specify backstep welding procedure 5. 100 = (1x 800)/ 2t t= 4 mm Page 17 of 23 Rev 1 .10) Longitudinal stress is half of hoop stress = 100/2 = 50 N/mm2 Hoop Stress = pd/2t Substituting the values in the above.2 Consider the following data for a thin-walled air receiver: Diameter (d) =800 mm Internal pressure (p) =10 bars Hoop stress =100 N/mm2 Find the wall thickness of the air receiver and the longitudinal stress. 10 marks (Ref: 3. All actions should have a procedure or instruction which will be referenced or indicated on the plan.1 List the three stages in the development of welding procedures. material type.3 (Ref: 4. The plan can also specify the extent of NDT of weld and who is to perform the inspection Page 18 of 23 Rev 1 . 4.1. In general. material thickness and edge preparation. • The proposed welding procedure • The procedure qualification record-PQR • The welding procedure specification. 4.2) 5 marks QUESTION 2 2. Route cards are used to assist further the planning and recording of work. The ITP integrates inspection activity and customer’s involvement with the production phases.2 5 marks A change in specified mean arc voltage A change in specified mean welding current A change in position in which the welding is done or change in welding direction A change from single pass to multipass A change in minimum specified preheat or inter-run temperature List the five methods of qualifying welding procedures available in AS/NZS 1554 Part1.WPS List five common essential variables for the MMAW process with reference to AS/NZS 1554 Part 1. wok should not proceed to the next stage until it has been inspected.1. 10 marks • A pre-qualified procedure • Production of documentary evidence of relevant prior experience by the fabricator • Production of a suitable length of test piece of the same joint type.2) 5 marks 1.PAPER SA4 FABRICATION AND APPLICATIONS ENGINEERING QUESTION 1 1.1 List three reasons for having an “Inspection and Test Plan (ITP)”. For smooth production and effective quality control it is necessary to plan for inspection and testing. material type and direction of rolling • Preparation of a special test piece • Destructive testing of a prototype joint • A welding procedure qualified by another fabricator (Ref: 4. • • • • • 1. 1 Give three reasons for lamellar tearing to occur.the shrinkage strains on welding must act in the short direction of the plate i. through the plate thickness 2. b) W 5 marks Fabrication is not to proceed until the manufacturer’s inspector has verified the performance and results of the inspection and test.1. Weld orientation .the plate must have poor ductility in the through-thickness direction Page 19 of 23 Rev 1 .e. 6 marks 1. QUESTION 3 (REF: 4.2. Material susceptibility .2 List ten components or elements of a typical ITP. Transverse strain .the fusion boundary will be roughly parallel to the plane of the inclusions 3. Material (at source of supply) Material (receipt) Component – mark out Fitup components Welder qualification Pressure testing Grit blasting Assembly Documentation Material testing Material cutting Component – flame cutting Weld procedures Welding Prior to painting Painting Packing & Dispatch 5 marks 2.2) 3. The inspector may delegate this authority to a suitable trained person whose training has been approved and recorded by the manufacturer.3 What is the intended action for the manufacturer's inspector when the following test points are specified in the ITP? a) H 5 marks Fabrication is not to proceed until manufacturer’s inspector has verified the performance and results of the inspection and test. 4. recommend an alternative joint configuration to reduce the risk of lamellar tearing 6 marks As tearing is more likely to occur in full penetration T butt joints. if possible.3. use two fillet welds b) Double-sided welds are less susceptible than large single-sided welds and balanced welding to reduce the stresses will further reduce the risk of tearing especially in the root Page 20 of 23 Rev 1 .2 a) For the welded joints given below. However. i) Excessive weld metal 4 marks Excessive weld metal which is usually a result of poor welder technique for manual processes but may be due to poor parameter selection when the process is mechanised. ii) Undercut 4 marks A wide spreading arc (high arc voltage) with insufficient fill (low current or high travel speed) is the usual cause. For mechanised techniques an increase in travel speed or voltage will help to reduce cap height. QUESTION 4 (REF: 4. High welding current will also cause undercut . If the imperfection is a result of welder technique then welder retraining is required. This imperfection may be avoided by reducing travel speed and/or the welding current and by maintaining the correct arc length. and the way the welding torch is angled can both cause and be used to overcome undercutting ( ie angled to push the weld metal to fill the melted groove). That is.3 Give two possible causes for each of the welding imperfections and one method of preventing each cause. as below. especially when weaving.3. welder technique.this is generally associated with the need for a high travel speed to avoid overfilling of the joint. 20 marks DATA • Weld Joint type: T joint • Single pass • Type of weld: Fillet (mitre) • Weld leg length: 6 mm Page 21 of 23 Rev 1 . too much filler metal for the travel speed used.8) 3.1 Calculate the labour cost and the filler material cost for a welding job given the following data. the diameter of the smallest wire that is visible to the eye under the correct lighting conditions is established.18 x 100 = 18 cm3 Weight of weld metal = Density x volume = 7.9 mm Deposition Efficiency = 95% Deposition Rate = 3.6 = 0.1487 x 5 = $ 0.6 = 4.85 x 18 / 1000 = 0.47 mins Labour hours = Arc on time / Operator factor = 2.85 x 103 kg/m3 Cost of filler material = $5/kg Hourly labour rate (including overhead) = $25 Operator Factor = 60% Area of cross section of electrode = ½ x base x height = ½ x 0.6 kg/hr Density of steel = 7. MMAW or powder technique can be used for buttering the edges of the joint followed by MMAW or GMAW/FCAW welding to fill the groove. To then calculate the IQI sensitivity of the radiograph.7435 Arc on time = Weld metal deposited/ Deposition rate = 0.13/60 x 25 = $1.72 QUESTION 5 5.47/0. 5.3 Page 22 of 23 Rev 1 .6 x 0.18 cm2 Volume of weld metal = area of cross section x length = 0.1413 kg Actual weld metal used = weight/ deposition efficiency = 0.9) 4 marks State two limitations of the ultrasonic inspection method Permanent record is difficult to obtain Requires high level of skill in interpreting indications How is the penetrameter used to determine the sensitivity of the radiograph? 4 marks In order to determine the sensitivity of a radiograph.13 mins Labour cost = Labour hours x Labour rate = 4. IQI are used as a means of assessing the image quality of the radiograph.1413/0. 4. a penetrameter or image quality indicator is used.• • • • • • • • • • Total weld length: 1000 mm Material: Carbon steel Welding Process: GMAW Wire diameter = 0. tables can be used as given in the National Standard or the diameter of the wire is divided by the weld thickness and then multiplied by 100 to give the sensitivity percentage List the general steps involved in the repairs of cast iron components for large areas 12 marks • For larger areas. For a wire laid across a weld.1487 kg Filler metal cost = Actual weld metal used x cost of filler material = 0.95 = 0.7.1487/3.6 x 60 = 2.1 • • 5.2 (REF: 4. • Remove defective area preferably by grinding or tungsten carbide burr. After gouging. If air arc or MMA gouging is used. Fill the groove using nickel (3 or 4mm diameter) or nickel-iron electrodes for greater strength. Preheat the casting to the required temperature Butter the surface of the groove with MMAW using a small diameter (2.4mm or 3mm) electrode. Finally. alternatively use oxy-acetylene with a powder consumable. the prepared area should be lightly ground to remove any hardened material. the weld area should be covered to ensure the casting will cool slowly to room temperature • • • • • • Page 23 of 23 Rev 1 . Remove slag and peen each weld bead whilst still hot. to avoid cracking through residual stresses. the component must be preheated locally to typically 300 degrees C. use a nickel or Monel rod to produce a soft. ductile 'buttered' layer.